Agnieszka Bondyra, Pawe Gotowicki


 Osborne Harris
 1 years ago
 Views:
Transcription
1 Journal of KONES Powertrain and Transport, Vol. 17, No INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON LAMINATE Agnieszka Bondyra, Pawe Gotowicki Military University of Technology Department of Mechanics & Applied Computer Science Gen. Sylwestra Kaliskiego 2 Street, 98 Warsaw tel.: , fax: Abstract The paper presents some experimental studies on a regular crossply laminate of the [(/9) F ] 4S configuration. Each layer is VE 11M vinylester resin (the manufacturer: OrganikaSarzyna Chemical Plants, Sarzyna, Poland) reinforced with pla in weave carbon fabric of parameters: S tyle 43, Carbon 6K, substance 3 g/m 2, warp/weft 4/4 tex, 3.7/ 3.7 yarn/cm (the manufacturer: C. Cramer GmbH & Co. KG Division ECC). The orthotropic laminate was produced by ROMA private enterprise in Grabowiec, Poland, using the vacuum molding method and the technological parameters developed by ROMA taking into account the VE 11M material specification. The PNEN ISO 14129:1997 standard [1] and closely related standards [29] were taken into consideration in experimental studies on the static inplane shear response by a tensile test of a [(±4) F ] ns laminate. A program of the experiments was focused on testing a rate of a testing machine crosshead and a number of sta tic stress cycles. An influence of these factors on the inplane shear modulus was investigated. Based on the conducted investigations, the modified experimental procedure has been proposed for determination of the correct value of the inplane shear modulus and the inplane shear strength. Keywords: vinylestercarbon laminate, regular crossply laminate,, inplane shear test, experimental procedure 1. Introduction Shear tests for polymermatrix composite materials are the most difficult tests for determining mechanical properties, particularly in the plane perpendicular to the laminate plane. There are wellknown numerous methods for shear tests of laminates. The most important of them are described below [113]. Two or three rails, which the specimens are attached to, are applied in the method of shear test in rails (ASTM D42/D42M1 [2]). This method defines the inplane shear modulus and the inplane shear strength. The length/width ratio for the measured region of the specimen is recommended to be greater than 1. The Iosipescu test method (ASTM D379/D379M [3]) uses fourpoint bending of the notched prismatic specimen. It allows determining the mechanical properties in all planes. Both methods require special instrumentation. The next method of a shear test applies a tensile test of a [(±4) F ] ns laminate (ISO 14129:2 [1] or its American equivalent ASTM D318/D318M94 [4]). This method allows determining the shear stress,, and the shear strain,, for polymermatrix composites with large failure deformations. It can be also used to determine the value of the inplane shear modulus, G 12, reliable since it is based on the straight section of the initial  relation. The plate torsion test (PNEN ISO 131:27 []) allows only determining the inplane shear modulus (G 12 ). The test uses simultaneous loading of the plate supported at two corners along its diagonal with cones placed at corners along the other diagonal.
2 A. Bondyra, P. Gotowicki Another method is a torsion test of a rod with circular or rectangular crosssection (PNC8976 [6]), with or without a hole. The method, for determining the apparent interlaminar shear strength of fiberreinforced composites using a short beam (PNEN ISO 1413:21 [7]), is applied to laminates with thermoset or thermoplastic matrix, under condition of damage caused by the interlaminar shear. This method can be applied to classify or to control the quality the materials. Standards related to the interlaminar shear strength of the plastics, developed separately for aviation and cosmonautics, are as follows: PNEN 2377:1994 [8] for glass fiberreinforced composites, and PNEN 263:2 [9] for unidirectional carbon fiberreinforced composites. Besides the abovementioned methods, there exist the others, such as: the tube twisting method (this method gives the most reliable results), the shear test using the fourbar linkage (the inplane shear; this method gives correct results for the inplane shear strength, but it is not suitable for determining the shear modulus), shear of a specimen in biaxial load (applied for many materials), torsion of ring specimens (applied in investigation of a pipeshaped laminate), shear of a specimen with notches (however, resulting in a large error) [12]. Originally, many of these test methods were dedicated to materials different from composites reinforced with continuous fibers (metals, wood, polymers). Some of them are not even standardized. Compatibility of these methods related to accuracy of determining the shear modulus is noted, whereas determining of the shear strength is more problematical. The edge effects, connecting of materials, nonlinear behaviour of the matrix or the matrixfibers connection, stress distribution (imperfections), existing of the normal stresses, cause that the value of the shear strength determined by existing methods is disputable. Therefore, the value of shear strength in engineering applications should be checked for each structure. Some of the test methods were proposed to determine the relation in a plane of the layer for fiberreinforced composites, the other ones are confined to the plane perpendicular to the previous one and some in dependence of cut of the specimen allow researching both cases. Summing up, the shear modulus and/or the shear strength are determined on the basis of the shear test. It is also possible to determine the failure strain. 2. Description of the experimental studies The aim of this study is to determine the influence of selected factors, i.e., a rate of the testing machine crosshead, a number of cycles of static stress, and sensors used for strain measurement, on the shear stress shear strain relation in the inplane shear test [1]. There is considered a vinylestercarbon regular crossply laminate denoted with the C/VE code. The modified procedure will be developed related to the test method presented in PNEN ISO standard [1]. It results from the fact that this standard does not take into account abovementioned factors Description of the test method The shear test method corresponds to the PNEN ISO standard [1] and permits to determine the shear stress,, and the shear strain,, of polymermatrix composites at large failure strain, without additional instrumentation. This method can be applied to determine the inplane shear modulus G 12. According to Ref. [1], the shear stress corresponding to % strain (if destruction of the specimen does not occur earlier) is assumed as a failure criterion. Such a criterion is also recommended by the ASTM D 318 standard [4]. According to Ref. [1], one load cycle is performed out at velocity given in a standard related to the tested material or 2 mm/min in case of lack of such data. Investigation was finished at =., if breaking of the specimen did not occur earlier. The shear modulus is defined in the interval of =.1., and the shear strength corresponds to the shear stress at the failure of the specimen or at =.. 3
3 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... The method uses a tensile test of a [(±4) F ] ns laminate and can be applied in case of laminates with thermosetting matrices. The method is not suitable for investigation of laminates reinforced with thick fabrics. It is sensitive to number and distribution of the layers; the comparison is made using the same number of layers. The laminate of the ±4 symmetrical configuration can be made of unidirectional or fabrics reinforced layers, provided that the number of fibers in the warp and the weft is equal to each other. During the tests, the specimen in the form of a rectangular beam with the fibers oriented at the angle of ±4 to the specimen axis is subjected to an axial tension load. The fibers should be arranged symmetrically and in a sustainable manner with respect to the specimen axis. It should be noted that the specimen material during the measurement is not in a state of pure shear, since in the ±4 system there occur both shear and normal stresses. Uptodate studies show that the normal stresses exhibit only negligible influence on the value of the shear modulus, G 12, and only slightly decrease the shear strength, R 12 [12] The tested material The tests were carried out for the C/VE regular crossply laminate of [(/9) F ] 4S configuration. The Style 43 fabric was produced by the ECC using carbon fibers TenaxE HTA4, with fiber parameters provided in Tab. 1. The fabric is characterized by the following parameters: Style 43, a plain weave,.42 mm thickness, 1 mm width, 3 g/m 2 substance, 4/4 warp/weft, 3.7/3.7 yarn/cm. The vinylester resin VE 11M applied for laminates with increased requirements for chemical resistance and incombustibility was used to manufacture the considered composite. The VE 11M resin parameters are given in Tab. 2. Prefabricated laminate plates used in the investigations were produced by ROMA private enterprise; they were made using the vacuum molding method and the technological parameters developed by ROMA taking into account the VE 11M datasheet. Tab. 1. Properties of the fiber (manufacturer data) L.P. Property Unit Value 1 Sizing  E13 (Epoxy) 2 The content of the roving preparation % Number of filaments  6K (6) 4 Nominal linear density tex 4 Filament diameter m 7 6 Density g/cm Tensile strength MPa 39 8 Young s modulus at tension GPa Elongation at break .17 Tab. 2. Properties of the resin matrix (manufacturer data) L.P. Property Unit Value Standard 1 Tensile strength MPa 8 ISO Young s modulus at tension GPa 3. ISO Elongation at break % 3. ISO Flexural strength MPa 12 ISO 178 Young s modulus at bending GPa 4 ISO Temperature of deflection under load C 8 ISO Barcol hardness B 4 ASTMD
4 A. Bondyra, P. Gotowicki 2.3. Preparation of specimens Plates of mm dimensions, made using the vacuum molding method, were cut into small [(±4) F ] ns plates of length equal to the test specimen and of width appropriate for preparation of the required number of specimens. Additional cover plates were prepared in a similar manner. The cover plates were glued to the plate using a thin layer of adhesive (E3 epoxy resin), according to [1]. The glued surfaces were degreased and sandpapered. The combined parts were tightened until the resin has been polymerized (12 h). Plates, together with the cover plates, constituted the initial material for cutting the specimens. Rectangular prism shaped specimens were cut using a sawing machine with a diamond disk. The mechanically machined surfaces and edges of final specimens were free of imperfections visible through a magnifying glass with a low magnification. Further processing was performed by milling. For roughing, made on the numerically controlled CNC BFN 7SERVO AUTO milling machine, the speed 1 rpm and feed rate 898 mm/min were used, and for the final treatment 1 rpm and 1224 mm/min, respectively. After the final treatment, the shape and dimensions of the specimens were compatible with standard [1] (Fig. 1, 2). Fig. 1. A shape and geometry of the specimen, according to Ref [1] Fig. 2. Specimens for the shear test According to Ref. [1], the formed shapes were conditioned for more than 88 hours at temperature of 23 ±1 C and relative humidity of ±1%. The tests were performed at the same conditions Instrumentation, measuring of the specimens, performing the tests A width of the specimens was measured using a calliper of.1 mm accuracy, a thickness measured of.1 mm accuracy using a micrometer with the 2 mm cylinder foot. The measurements 32
5 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... were executed in accordance with Ref. [1]. Afterwards, the arithmetic mean of three measurement results was calculated. Longer edges of individual specimens were parallel with tolerance of.2 mm, therefore, respective standard requirements were fulfilled. The investigations were executed on the INSTRON 882 universal testing machine with hydraulic wedge grips (Fig. 3). Fig. 3. View of a specimen mounted in the hydraulic wedge grips Four different crosshead rates were used during the tests: 1, 2, and 1 mm/min. The circuit of the load measurement showed the total spreading load transferred by the specimen and it did not show the inertial deceleration at every applied crosshead rate. Using the FastTrack software, the measured values of displacement, force and deformation in real time were automatically recorded and saved on a hard disk with sampling frequencies of, 1, 2 and Hz, respectively. The measurement of deformation was performed in two directions, i.e., parallel and perpendicular to the axis of the specimen. Vishay strain gauges of the a6 mm measuring base, 12 resistance, sensitivity constant k = 2.8, and two extensometers axial, INSTRON , and transverse, INSTRON WE44E, were used, both of the 2 mm measuring base (Fig. 4). a) b) Fig. 4. A specimen with installed sensors: a) strain gauges b) extensometers 33
6 2.. Processing of the measurement results [1] A. Bondyra, P. Gotowicki The shear stress was calculated using the formulas resulting from rotation about the angle of 4 in uniaxial tension: F 12 ( F),,, (1) bh where: 12  the current inplane shear stress [MPa], F  the current load [N], b  width of the specimen [mm], h  thickness of the specimen [mm]. The inplane shear strength is equal to R ( Fm ), (2) where: F m  load at break of the specimen or load corresponding to the deformation 12 =., if the test was completed before the specimen s failure [N], R 12  the inplane shear strength (maximum shear stress before the moment of completion of the test or at the deformation 12 =.) [MPa]. The shear strain is determined from the formula resulting from the deformation in uniaxial tension and rotation about the angle of 4 in the layer plane, i.e., 12 x y, (3) where: 12  shear strain (total deformation related to the directions parallel and perpendicular to the axis of the specimen), x, y  normal strains in the directions parallel and perpendicular to the axis of the specimen ( x >, y <). The shear modulus is calculated from the initial quasilinear shear stress shear strain relation: 12'' 12' G, 12 (4) 12'' 12' where: G 12  shear modulus [GPa], 12  shear stress corresponding to the strain of 12 =.1, 12  shear stress corresponding to the strain of 12 =., The shear stress shear strain relation was determined for each specimen. 3. Test results and their analysis Evaluation of the usefulness of sensors used for strain measurements A comparative study was carried out in order to evaluate the usefulness of sensors for the strain measurement. Extensometers and strain gauges were installed on the same specimen (Fig. 4). Figure shows the results of the measurement using strain gauges and extensometers versus time, at the rate of crosshead v = 1 mm/min. Significant differences in the strain recorded by the axial and transverse strain gauges and similar values of the strain recorded by the axial and transverse extensometers can be observed. This is caused by the stress distribution in the specimen. Strain gauges measured the strain in a small area close to the axis of the specimen, whereas extensometers measured the strain of the region covering the entire width of the specimen (gauges base 6 mm, extensometers 34
7 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... base 2 mm). The strain is the sum of the absolute values of strains x, y and the strain for both types of sensors, calculated in this way, will be similar. The disadvantage of strain gauges is found in a smaller range of measured strain and in lack of reusability. The advantage of extensometers is averaging of shear strains in a large area of the specimen, ease and simplicity of installation. The test (Fig. ) ends at time t 14 s which corresponds to strain value of =.. Values recorded by a transverse strain gauge at the moments of t 24 and 27 s, are caused by shortcircuiting. Taking into account the above preliminary analysis, only extensometers were used in further experiments.,3,3,2,2 [],1,1, Transverse strain gauge Axial strain gauge Transverse extensometer Axial extensometer t [s] Fig.. Strains versus time recorded by strain gauges and extensometers for the selected specimen 3.2. Results of the measurements and their analysis In order to determine influences of a rate of the testing machine crosshead and of a number of stress cycles on the static relationship , the loading program presented in Fig. 6 was assumed. Each specimen was subjected to five cycles of kinematic loading of a triangular shape, at intervals of 3' that protect finishing the reverse creep after each cycle. Each cycle contains a linear increase of the vertical displacement of the traverse up to. mm ( =..6) and a linear decrease to zero. Fig. 6. The loading program for testing selected factors in the shear test The kinematic loading was executed at constant speed v = 1, 2, or 1 mm/min of the traverse. In this way, four fivecycle  diagrams for subsequent specimens were obtained, as shown in Figs
8 A. Bondyra, P. Gotowicki 2 2 v=1 mm/min 1 [MPa] 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 7. The  diagram for v = 1 mm/min (specimen No. 8) 2 2 v=2 mm/min 1 [MPa] 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 8. The  diagram for v = 2 mm/min (specimen No. 9) 2 2 v = mm/min 1 [MPa] 1  cycle 1 cycle 2 cycle 3 cycle 4 cycle,1,2,3,4,,6 Fig. 9. The  diagram for v = mm/min (specimen No. 1) 36
9 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for v=1 mm/min [MPa] 1 1 cycle 1 cycle 2 cycle 3 cycle 4 cycle ,1,2,3,4,,6 Fig. 1. The  diagram for v = 1 mm/min (specimen No. 11) Analysis of the  hysteresis loops presented in Figs. 71 leads to the following conclusions: 1) The executed strain interval corresponds to a linear Hooke's law. Small curvatures of plots in each cycle and a hysteresis loop indicate the occurrence of viscoelastic strains nonnegligible for the tested crosshead rates and the stress range. Viscoelastic strains in the loading test are typical for laminates [14]. Evidence of this phenomenon is observed in the graph of the load versus time in the first cycle at v = 1 mm/min (specimen No. 8), shown in Fig. 11 and in the graph of the  diagram shown in Fig. 12 for the strain range of =.1. proposed by ISO [1] in order to determine the shear module. 2) Along with increase of the crosshead rate a width of the hysteresis loop decreases. It corresponds to decrease of rheological effects. 3) After the first load cycle the permanent strain of ~.2 value occurs. This strain corresponds to redistribution of the residual stresses in the laminate caused by the manufacture technology. During the stress increase in the first load cycle, there appear microcracks in the laminate, distributed quasiuniformly in the whole volume of the specimen. 4) In the second and subsequent load cycles, the permanent strain increase is negligible. Therefore, in the 2 nd, 3 rd, 4 th, th load cycles, further degradation of the laminate microstructure does not occur. ) In the interval =.1.2, the  relationship is quasilinear for the tested traverse velocities, and thus the viscoelastic strains in this interval can be neglected (Fig. 13). 3, 2, 2, [kn] load 1, 1, v=1 mm/min, cycle 1,, , time [s] Fig. 11. The axial tensioning force versus time for v = 1 mm/min in cycle 1 (specimen No. 8) 37
10 A. Bondyra, P. Gotowicki 2 2 [MPa] 1 1 v=1 mm/min, cycle 1,1,2,3,4, Fig. 12. The  diagram for v = 1 mm/min in a cycle 1oad its linear regression for =.1. (specimen 8) 2 2 [MPa] 1 1 v=1 mm/min, cycle 1,1,2,3,4, Fig. 13. The  diagram for v = 1 mm/min in a cycle 1oad its linear regression for =.1.2 (specimen 8) The values of the shear modulus, G 12, for subsequent cycles of kinematic loading and applied load rates, calculated on the basis of the quasilinear strain interval =.1.2, are presented in Tab. 3 and Fig. 14. Tab. 3. The shear modulus calculated for the strain interval =,1,2 Specimen No. v G 12 [GPa] [mm/min] cycle 1 cycle 2 cycle 3 cycle 4 cycle The values of the shear modulus, G 12, at the 2 nd, 3 rd and 4 th load cycles can be considered as independent of the velocity of the crosshead rate and of a number of the loading cycles. In the first cycle, the shear modulus is greater by 6.4% (an average value) when compared to the second cycle results. 38
11 Influence of a Crosshead Rate and a Number of Stress Cycles on Measurement Results in the InPlane Shear Test for... 4 G 12 [GPa] mm/min 2 mm/min mm/min 1 mm/min cycle Fig. 14. The dependence of the shear modulus on a number of the loading cycles and on the crosshead rate 4. Final conclusions Taking into account notation in the PNEN ISO standard [1] and detailed conclusions resulting from the experiments, the authors propose the following modified procedure concerning determination of selected mechanical properties of orthotropic laminates in the inplane shear test: 1) Execution of the initial loading cycle of the triangular shape (linear increase of the crosshead displacement up to. mm and a linear decrease to zero), at the crosshead rate of v = 2 mm/min) in order to redistribute the residual (technological) stresses in the specimen. 2) A 3 break after the initial loading cycle, in order to perform the reverse creep of the specimen. 3) Execution of the main test, i.e., linear increase of the crosshead displacement at the velocity of v = 2 mm/min until the break of the specimen appears or the limited strain =. is reached. Determination of the  diagram. 4) Determination of the shear modulus G 12 based on the =.1.2 interval, using the linear regression due to measurement fluctuations. ) Determination of the shear strength R 12 equal to the maximum value in the  diagram. Other requirements formulated in Ref. [1], related to the specimen s preparation and conditioning, the experiment performing and processing of the measurement results, are fully accepted and applied in this study. References [1] PNEN ISO 14129:2, Material composites reinforced with a fib re. Determination of th e shear stress and the respective strain, shear modulus and shear strength in the in plane shear test by a tensile test of a ±4 laminate [in Polish]. [2] ASTM D42/D42M1:27, Standard test method for inplane shear properties of polymer matrix composite materials by the Rail Shear Method. [3] ASTM D379/D379M:1998, Standard test method for shear properties of composite materials by the VNotched Beam Method. [4] ASTM D318/D318M94:27, Standard test method for inplane shear response of polymer matrix composite materials by tensile test of a ±4 laminate [] PNEN ISO 131:27, Material composites reinforced with a fib re. Determination of th e inplane shear modulus using the plate torsion method [in Polish]. [6] PNC8976:1974, Plastics, Determination of a temperature dependent shear modulus at torsion [in Polish]. 39
12 A. Bondyra, P. Gotowicki [7] PNEN ISO 1413:21, Material composites reinforced with a fib re. Determination of th e conventional interlaminar shear strength using the short beam method [in Polish]. [8] PNEN 2377:1994, Aeronautics and cosmonautics. Plastics rein forced with g lass fibres. A method for determination of conventional interlaminar shear strength [in Polish]. [9] PNEN 263:2, Aeronautics and cosmonautics. Plastics reinforced with carbon fibres. Unidirectional laminates. Determin ation of co nventional interlaminar shear strength [in Polish]. [1] Tarnopol skii, Y. M., Arnautov, A. K. and Kulakov, V. L.: Methods of determination of shear properties of textile composites. Composites Part A, Applied Science and Manufacturing Vol. 3, No. 7, pp , [11] Van Paepegem, W., De Baere, I., Degrieck, J., Modelling the nonlinear shear stress strain response of glass fibrereinforced composites, Part I, Experimental results, Composites Science and Technology, Vol. 66, No. 1, pp , 26. [12] Ochelski, S., Experimental methods in mechanics of structural composites [in Polish], WNT, 24. [13] Miracle, D. B., Donaldson, S. L., ASM Handbook, Vol. 21: Composites, ASM International, 21. [14] Klasztorny, M., Niezgoda, T., Viscoelastic modeling of regu lar crossply laminates, Kompozyty (Composites), Vol. 9, No. 3, pp , 28. Acknowledgements This work is a part of a project No. O R 62 6 funded in by Ministry of Science and Higher Education, Poland. This support is gratefully acknowledged. The work was supervised by Professor M. Klasztorny, PhD, DSc, Military University of Technology, Warsaw, Poland. 4
Flexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationHIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS HIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES Warnet L., Akkerman R., Ravensberg M. University of Twente, Faculty of Engineering Technology,
More informationGB/T / ISO 5271:1993
Translated English of Chinese Standard: GB/T1040.12006 www.chinesestandard.net Sales@ChineseStandard.net GB NATIONAL STANDARD OF THE PEOPLE S REPUBLIC OF CHINA ICS 83.080.01 G 31 GB/T 1040.12006 / ISO
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationDEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL
DEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL S. Quinn*, R.K. Fruehmann and J.M. DulieuBarton School of Engineering Sciences University of Southampton Southampton SO17
More informationMATERIALS AND METHODS
Modelling the Nonlinear Shear Stress Strain Behavior of a Carbon Fabric Reinforced Polyphenylene Sulphide From Rail Shear and [(458,2458)] 4s Tensile Test Ives De Baere, Wim Van Paepegem, Joris Degrieck
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationThe influence of fiber undulation on the mechanical properties of FRPlaminates. Christian Fiebig, Michael Koch
URN (Paper): urn:nbn:de:gbv:ilm12014iwk099:3 58 th ILMENAU SCIENTIFIC COLLOQUIUM Technische Universität Ilmenau, 08 12 September 2014 URN: urn:nbn:de:gbv:ilm12014iwk:3 The influence of fiber undulation
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationComposite Materials Research Laboratory, State University of New York at Buffalo, Buffalo, NY , USA
Composite Interfaces, Vol. 7, No. 4, pp. 257 275 (2000) VSP 2000. Discontinuous surfacetreated submicrondiameter carbon filaments as an interlaminar filler in carbon fiber polymermatrix composites for
More informationISO 178 INTERNATIONAL STANDARD. Plastics Determination of flexural properties. Plastiques Détermination des propriétés en flexion
INTERNATIONAL STANDARD ISO 178 Fourth edition 20011215 Plastics Determination of flexural properties Plastiques Détermination des propriétés en flexion Reference number ISO 2001 PDF disclaimer This PDF
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationPDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [ ] Introduction, Fundamentals of Statics
Page1 PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [2910601] Introduction, Fundamentals of Statics 1. Differentiate between Scalar and Vector quantity. Write S.I.
More informationDEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION
DEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION B. Zhu 1,2*, T.X. Yu 1, X.M. Tao 2 1 Department of Mechanical Engineering, Hong Kong University of Science
More informationUSE OF DIGITAL IMAGE CORRELATION TO OBTAIN MATERIAL MODEL PARAMETERS FOR COMPOSITES
USE OF DIGITAL IMAGE CORRELATION TO OBTAIN MATERIAL MODEL PARAMETERS FOR COMPOSITES Brian Croop, Hubert Lobo (DatapointLabs, USA). Presenter: Hubert Lobo, President SUMMARY The development of material
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationStrain Measurement. Prof. Yu Qiao. Department of Structural Engineering, UCSD. Strain Measurement
Strain Measurement Prof. Yu Qiao Department of Structural Engineering, UCSD Strain Measurement The design of loadcarrying components for machines and structures requires information about the distribution
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationTENSILE TESTS (ASTM D 638, ISO
MODULE 4 The mechanical properties, among all the properties of plastic materials, are often the most important properties because virtually all service conditions and the majority of enduse applications
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationNUMERICAL SIMULATION OF BLAST RESISTANT STEEL PLATE STRENGTHENED WITH COMPOSITE
Journal of KONES Powertrain and Transport, Vol. 18, No. 3 2011 NUMERICAL SIMULATION OF BLAST RESISTANT STEEL PLATE STRENGTHENED WITH COMPOSITE Krzysztof Kosiuczenko, Tadeusz Niezgoda, Wies aw Barnat, Robert
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationEFFECTS OF TEMPERATURE AND ENVIRONMENT ON MECHANICAL PROPERTIES OF TWO CONTINUOUS CARBON FIBER AUTOMOTIVE STRUCTURAL COMPOSITES. M. B.
ORNL/TM2003/117 EFFECTS OF TEMPERATURE AND ENVIRONMENT ON MECHANICAL PROPERTIES OF TWO CONTINUOUS CARBON FIBER AUTOMOTIVE STRUCTURAL COMPOSITES M. B. RugglesWrenn DOCUMENT AVAILABILITY Reports produced
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationNAME: Given Formulae: Law of Cosines: Law of Sines:
NME: Given Formulae: Law of Cosines: EXM 3 PST PROBLEMS (LESSONS 21 TO 28) 100 points Thursday, November 16, 2017, 7pm to 9:30, Room 200 You are allowed to use a calculator and drawing equipment, only.
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationCHARACTERISATION OF FIBRE GLASS PANELS FOR NAVAL USE
ICEM1212th International Conference on Experimental Mechanics 29 August  2 September, 2004 Politecnico di Bari, Italy CHARACTERISATION OF FIBRE GLASS PANELS FOR NAVAL USE D. Lombardo a, G. Marannano
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationReliable Test Results
Intelligent testing Johannes J.Bührle  Agenda Reliable test results are a fundamental and highly topical aspect of materials testing. Using suitable examples we would like to show you how we view this
More informationSCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL
SCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL LAMINATES J. G. Carrillo 1, S. McKown 1, M. Mujib 1 and W. J. Cantwell 1. R. Day 2 1 Department of Engineering, University of Liverpool,
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationElastic Properties of Solids (One or two weights)
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids (One or two weights) This is a rare experiment where you will get points for breaking a sample! The recommended textbooks and other
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationStress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus. Case study
Stress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus Case study 2 In field of Physics, it explains how an object deforms under an applied force Real rigid bodies are elastic we can
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationAnalysis of nonlinear shear deformations in CFRP and GFRP textile laminates
Loughborough University Institutional Repository Analysis of nonlinear shear deformations in CFRP and GFRP textile laminates This item was submitted to Loughborough University's Institutional Repository
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More informationMassachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA Problem Set 14
Massachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA 02139 16.01/16.02 Unified Engineering I, II Fall 2003 Problem Set 14 Name: Due Date: 12/9/03 F18 F19 F20 M19
More informationMechanics of Materials
Mechanics of Materials Notation: a = acceleration = area (net = with holes, bearing = in contact, etc...) SD = allowable stress design d = diameter of a hole = calculus symbol for differentiation e = change
More informationFOLDING OF WOVEN COMPOSITE STRUCTURES
FOLDING OF WOVEN COMPOSITE STRUCTURES J.C.H. Yee and S. Pellegrino 1 Department of Engineering, University of Cambridge Trumpington Street, Cambridge CB2 1PZ, UK ABSTRACT This paper investigates oneply
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationALIGNED FLAX FIBRE/POLYLACTATE COMPOSITES A MATERIALS MODEL SYSTEM TO SHOW THE POTENTIAL OF BIOCOMPOSITES IN ENGINEERING APPLICATIONS
ALIGNED FLAX FIBRE/POLYLACTATE COMPOSITES A MATERIALS MODEL SYSTEM TO SHOW THE POTENTIAL OF BIOCOMPOSITES IN ENGINEERING APPLICATIONS Bo Madsen 1, Hans Lilholt 1, Anders Thygesen 2, Elaine Arnold 3, Brendon
More informationNUMERICAL ANALYSIS OF PROGRESSIVE FAILURE OF COMPOSITE ENERGY ABSORBING STRUCTURES
Journal of KONES Powertrain and Transport, Vol. 15, No. 1 008 NUMERICAL ANALYSIS OF PROGRESSIVE FAILURE OF COMPOSITE ENERGY ABSORBING STRUCTURES Tadeusz Niezgoda, Wiesaw Barnat Military University of Technology
More informationMassachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA Problem Set 14
Massachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA 02139 16.01/16.02 Unified Engineering I, II Fall 2003 Problem Set 14 Name: Due Date: 12/9/03 F18 F19 F20 M19
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationCIVIL DEPARTMENT MECHANICS OF STRUCTURES ASSIGNMENT NO 1. Brach: CE YEAR:
MECHANICS OF STRUCTURES ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes XX and YY of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationDESIGNING A FLEXIBLE BELLOWS COUPLING MADE FROM COMPOSITE MATERIALS USING NUMERICAL SIMULATIONS SVOČ FST 2018
DESIGNING A FLEXIBLE BELLOWS COUPLING MADE FROM COMPOSITE MATERIALS USING NUMERICAL SIMULATIONS SVOČ FST 2018 Ing. Frantisek Sedlacek, University of West Bohemia, Univerzitni 8, 306 14, Pilsen, Czech Republic
More informationMechanical behaviour of wood in the orthotropic directions
Mechanical behaviour of wood in the orthotropic directions J.. Morais 1, J. C. Xavier 1, N. M. Dourado 1, J.. ousada 2 1 Departamento de Engenharias, ICETA/UTAD, Portugal 2 Departamento de Florestal, ICETA/UTAD,
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationSabah Shawkat Cabinet of Structural Engineering Walls carrying vertical loads should be designed as columns. Basically walls are designed in
Sabah Shawkat Cabinet of Structural Engineering 17 3.6 Shear walls Walls carrying vertical loads should be designed as columns. Basically walls are designed in the same manner as columns, but there are
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationGEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE
GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.02225767328 email: cejnm@civil.iitb.ac.in Module13 LECTURE
More informationBioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test
BioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test Objectives 1. To be familiar with the material testing machine(810le4) and provide a practical
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More information2. (a) Explain different types of wing structures. (b) Explain the advantages and disadvantages of different materials used for aircraft
Code No: 07A62102 R07 Set No. 2 III B.Tech II Semester Regular/Supplementary Examinations,May 2010 Aerospace Vehicle Structures II Aeronautical Engineering Time: 3 hours Max Marks: 80 Answer any FIVE
More informationFIS Specifications for Flex Poles (Edition May 2008) Original Text: German
FIS Specifications for Flex Poles (Edition May 2008) Original Text: German 1 Field of Application and Basic Information The following FIS specifications for flex poles are intended to ensure that flex
More informationConsider an elastic spring as shown in the Fig.2.4. When the spring is slowly
.3 Strain Energy Consider an elastic spring as shown in the Fig..4. When the spring is slowly pulled, it deflects by a small amount u 1. When the load is removed from the spring, it goes back to the original
More informationSTRAIN GAUGES YEDITEPE UNIVERSITY DEPARTMENT OF MECHANICAL ENGINEERING
STRAIN GAUGES YEDITEPE UNIVERSITY DEPARTMENT OF MECHANICAL ENGINEERING 1 YEDITEPE UNIVERSITY ENGINEERING FACULTY MECHANICAL ENGINEERING LABORATORY 1. Objective: Strain Gauges Know how the change in resistance
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More information